#------------------------------------------------------------------------------
#$Date: 2016-02-14 06:40:26 +0200 (Sun, 14 Feb 2016) $
#$Revision: 176432 $
#$URL: svn://www.crystallography.net/cod/cif/2/10/22/2102204.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2102204
loop_
_publ_author_name
'Norberg, Stefan T.'
'Streltsov, Victor A.'
'Svensson, Göran'
'Albertsson, Jörgen'
_publ_section_title
;
 Dopant positions in strontium/chromium- and barium-doped KTP,
 determined with synchrotron X-radiation
;
_journal_coeditor_code           OS0060
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              980
_journal_page_last               987
_journal_paper_doi               10.1107/S0108768100012866
_journal_volume                  56
_journal_year                    2000
_chemical_formula_moiety         'Ba0.06 K0.88 Ti O P O4'
_chemical_formula_sum            'Ba0.06 K0.88 O5 P Ti'
_chemical_formula_weight         201.6
_space_group_IT_number           33
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'P 2c -2n'
_symmetry_space_group_name_H-M   'P n a 21'
_cell_angle_alpha                90.000
_cell_angle_beta                 90.000
_cell_angle_gamma                90.000
_cell_formula_units_Z            8
_cell_length_a                   12.851(6)
_cell_length_b                   6.418(3)
_cell_length_c                   10.620(5)
_cell_measurement_reflns_used    12
_cell_measurement_temperature    120(1)
_cell_measurement_theta_max      45.0
_cell_measurement_theta_min      25.3
_cell_volume                     875.9(7)
_computing_cell_refinement       'BL14A (Tsukuba, Japan)'
_computing_data_collection       'BL14A (Tsukuba, Japan)'
_computing_data_reduction
'Xtal3.6 (Hall et al., 1999) DIFDAT ADDREF ABSORB SORTRF'
_computing_molecular_graphics
;ORTEPIII (Burnett & Johnson, 1996) and Xtal3.6 (Hall et al., 1999) FOURR
 SLANT
CONTRS
;
_computing_publication_material
'Xtal3.6 (Hall et al., 1999) BONDLA ATABLE CIFIO'
_computing_structure_refinement  'Xtal3.6 (Hall et al., 1999) CRYLSQ'
_diffrn_ambient_temperature      120(1)
_diffrn_measurement_device_type  'bl14a 4-circle'
_diffrn_measurement_method       ω-2θ
_diffrn_radiation_detector       'avalanche photo diode'
_diffrn_radiation_monochromator  si(111)
_diffrn_radiation_source         'photon factory bl14a'
_diffrn_radiation_type           'synchrotron x-ray vertical wiggler'
_diffrn_radiation_wavelength     .75000(9)
_diffrn_reflns_av_R_equivalents  .079
_diffrn_reflns_av_sigmaI/netI    .059
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            10098
_diffrn_reflns_reduction_process 'equatorial monochr Lp'
_diffrn_reflns_theta_max         32.38
_diffrn_reflns_theta_min         3.35
_diffrn_standards_decay_%        2
_diffrn_standards_interval_count 94
_diffrn_standards_number         6
_exptl_absorpt_coefficient_mu    3.605
_exptl_absorpt_correction_T_max  .9446
_exptl_absorpt_correction_T_min  .8959
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
Alcock, N. W. 1974. Absorption and Extinction Corrections: Calculation
Methods and Standard Tests. Acta Cryst. A30, 332-335
;
_exptl_crystal_colour            'light green-brown'
_exptl_crystal_density_diffrn    3.057
_exptl_crystal_density_meas      ?
_exptl_crystal_description       prism
_exptl_crystal_F_000             776.86
_exptl_crystal_size_max          0.032
_exptl_crystal_size_mid          0.024
_exptl_crystal_size_min          0.016
_refine_diff_density_max         .722
_refine_diff_density_min         -.721
_refine_ls_abs_structure_details 'Flack xabs refined'
_refine_ls_abs_structure_Flack   0.56(5)
_refine_ls_extinction_coef       8997(2536)
_refine_ls_extinction_expression 'Eq22 p292 "Cryst. Comp." Munksgaard 1970'
_refine_ls_extinction_method     'Gaussian (Zachariasen, 1967)'
_refine_ls_goodness_of_fit_all   3.34
_refine_ls_goodness_of_fit_ref   2.97
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     150
_refine_ls_number_reflns         2631
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          .033
_refine_ls_R_factor_gt           .031
_refine_ls_shift/su_max          .001
_refine_ls_shift/su_mean         .0001
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/σ²(F)
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         .051
_refine_ls_wR_factor_ref         .045
_reflns_d_resolution_high        .7
_reflns_d_resolution_low         6.417
_reflns_Friedel_coverage         .906
_reflns_limit_h_max              18
_reflns_limit_h_min              0
_reflns_limit_k_max              9
_reflns_limit_k_min              0
_reflns_limit_l_max              15
_reflns_limit_l_min              -15
_reflns_number_gt                2631
_reflns_number_total             2663
_reflns_threshold_expression     F>2σ(F)
_cod_data_source_file            os0060.cif
_cod_data_source_block           BaKTP
_cod_depositor_comments
;
The following automatic conversions were performed:

'_chemical_melting_point' value 'not measured' was changed to '?' -
the value is undefined or not given.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 

The following automatic conversions were performed:

'_chemical_melting_point' value 'not measured' was changed to '?' -
the value is undefined or not given.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        876.0(7)
_cod_original_sg_symbol_Hall     'p 2c -2n'
_cod_database_code               2102204
loop_
_symmetry_equiv_pos_as_xyz
+x,+y,+z
-x,-y,1/2+z
1/2-x,1/2+y,1/2+z
1/2+x,1/2-y,+z
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
K1 .37678(11) .2210(2) .30754(18) .0081(6) Uani 1.000(4)
K2 .1073(11) .300(2) .0568(13) .007(2) Uani 0.755(10)
Ba2 .104(2) .305(4) .069(2) .006(3) Uiso 0.123(3)
Ti1 .37269(8) .50034(16) .00013(17) .0038(4) Uani 1.00000
Ti2 .24644(9) .73294(16) .25070(16) .0035(4) Uani 1.00000
P1 .49818(13) .6639(2) .2582(2) .0030(6) Uani 1.00000
P2 .18075(11) .4977(2) .5104(2) .0032(6) Uani 1.00000
O1 .4863(4) .5128(7) .1485(4) .006(2) Uani 1.00000
O2 .5098(4) .5347(8) .3815(4) .005(2) Uani 1.00000
O3 .4003(4) .8019(7) .2769(4) .006(2) Uani 1.00000
O4 .5937(3) .8077(7) .2389(4) .0044(19) Uani 1.00000
O11 .2752(4) .5333(7) .1403(4) .005(2) Uani 1.00000
O12 .2238(4) .9586(8) .3873(4) .005(2) Uani 1.00000
O5 .1118(4) .6887(7) .5385(4) .005(2) Uani 1.00000
O6 .1110(4) .3085(7) .4852(4) .006(2) Uani 1.00000
O7 .2530(4) .4608(8) .6259(4) .006(2) Uani 1.00000
O8 .2530(4) .5388(8) .397(3) .005(2) Uani 1.00000
loop_
_atom_type_symbol
_atom_type_oxidation_number
_atom_type_number_in_cell
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
K 0 7.020 .1958 .2781 'Int Tables Vol IV Tables 2.2B and 2.3.1'
Ba 0 0.492 -.5402 2.5117 'Int Tables Vol IV Tables 2.2B and 2.3.1'
Ti 0 8 .2647 .4951 'Int Tables Vol IV Tables 2.2B and 2.3.1'
P 0 8 .1003 .1055 'Int Tables Vol IV Tables 2.2B and 2.3.1'
O 0 40 .0093 .0068 'Int Tables Vol IV Tables 2.2B and 2.3.1'
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
0 0 4
0 0 -4
0 4 0
0 -4 0
8 0 0
-8 0 0
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
K2 K1 Ba2 . . . 1.8(4) no
K2 K1 Ti1 . . . 53.31(18) no
K2 K1 Ti2 . . '1 545' 68.48(18) no
K2 K1 P1 . . . 100.21(19) no
K2 K1 P2 . . '3 544' 48.96(18) no
K2 K1 O1 . . . 87.4(2) no
K2 K1 O2 . . . 125.2(2) no
K2 K1 O3 . . '1 545' 97.4(2) no
K2 K1 O11 . . . 38.4(2) no
K2 K1 O12 . . '1 545' 72.0(2) no
K2 K1 O5 . . '3 544' 56.3(2) no
K2 K1 O7 . . '3 544' 41.4(2) no
K2 K1 O8 . . . 70.6(5) no
K2 K1 Ti2 . . . 56.46(18) no
K2 K1 K2 . . '3 545' 123.3(3) no
K2 K1 Ba2 . . '3 545' 124.5(4) no
K2 K1 K2 . . 3 107.0(3) no
K2 K1 Ba2 . . 3 108.0(4) no
K2 K1 K2 . . 4 100.6(3) no
K2 K1 Ba2 . . 4 101.7(4) no
Ba2 K1 Ti1 . . . 54.5(3) no
Ba2 K1 Ti2 . . '1 545' 68.7(3) no
Ba2 K1 P1 . . . 100.5(3) no
Ba2 K1 P2 . . '3 544' 50.6(3) no
Ba2 K1 O1 . . . 88.4(3) no
Ba2 K1 O2 . . . 125.1(3) no
Ba2 K1 O3 . . '1 545' 98.1(3) no
Ba2 K1 O11 . . . 38.6(3) no
Ba2 K1 O12 . . '1 545' 71.1(3) no
Ba2 K1 O5 . . '3 544' 58.1(3) no
Ba2 K1 O7 . . '3 544' 42.3(3) no
Ba2 K1 O8 . . . 69.1(6) no
Ba2 K1 Ti2 . . . 55.7(3) no
Ba2 K1 K2 . . '3 545' 122.5(4) no
Ba2 K1 Ba2 . . '3 545' 123.7(5) no
Ba2 K1 K2 . . 3 105.8(4) no
Ba2 K1 Ba2 . . 3 106.8(5) no
Ba2 K1 K2 . . 4 102.3(4) no
Ba2 K1 Ba2 . . 4 103.4(5) no
Ti1 K1 Ti2 . . '1 545' 105.37(6) no
Ti1 K1 P1 . . . 56.67(5) no
Ti1 K1 P2 . . '3 544' 53.93(5) no
Ti1 K1 O1 . . . 35.13(10) no
Ti1 K1 O2 . . . 84.65(10) no
Ti1 K1 O3 . . '1 545' 111.83(11) no
Ti1 K1 O11 . . . 31.52(10) no
Ti1 K1 O12 . . '1 545' 124.06(11) no
Ti1 K1 O5 . . '3 544' 33.13(9) no
Ti1 K1 O7 . . '3 544' 72.63(10) no
Ti1 K1 O8 . . . 86.4(5) no
Ti1 K1 Ti2 . . . 55.18(4) no
Ti1 K1 K2 . . '3 545' 163.1(2) no
Ti1 K1 Ba2 . . '3 545' 164.6(4) no
Ti1 K1 K2 . . 3 96.70(18) no
Ti1 K1 Ba2 . . 3 97.8(3) no
Ti1 K1 K2 . . 4 56.0(2) no
Ti1 K1 Ba2 . . 4 57.1(4) no
Ti2 K1 P1 '1 545' . . 161.17(8) no
Ti2 K1 P2 '1 545' . '3 544' 53.29(4) no
Ti2 K1 O1 '1 545' . . 133.80(12) no
Ti2 K1 O2 '1 545' . . 166.26(12) no
Ti2 K1 O3 '1 545' . '1 545' 34.28(10) no
Ti2 K1 O11 '1 545' . . 106.34(11) no
Ti2 K1 O12 '1 545' . '1 545' 34.82(11) no
Ti2 K1 O5 '1 545' . '3 544' 78.11(10) no
Ti2 K1 O7 '1 545' . '3 544' 33.21(10) no
Ti2 K1 O8 '1 545' . . 115.64(12) no
Ti2 K1 Ti2 '1 545' . . 121.94(6) no
Ti2 K1 K2 '1 545' . '3 545' 61.5(2) no
Ti2 K1 Ba2 '1 545' . '3 545' 63.2(4) no
Ti2 K1 K2 '1 545' . 3 145.64(18) no
Ti2 K1 Ba2 '1 545' . 3 145.3(3) no
Ti2 K1 K2 '1 545' . 4 101.7(2) no
Ti2 K1 Ba2 '1 545' . 4 101.7(4) no
P1 K1 P2 . . '3 544' 107.88(7) no
P1 K1 O1 . . . 27.65(10) no
P1 K1 O2 . . . 28.16(10) no
P1 K1 O3 . . '1 545' 141.47(12) no
P1 K1 O11 . . . 62.03(11) no
P1 K1 O12 . . '1 545' 158.06(12) no
P1 K1 O5 . . '3 544' 83.09(10) no
P1 K1 O7 . . '3 544' 129.29(12) no
P1 K1 O8 . . . 71.9(2) no
P1 K1 Ti2 . . . 54.99(5) no
P1 K1 K2 . . '3 545' 134.7(2) no
P1 K1 Ba2 . . '3 545' 133.1(4) no
P1 K1 K2 . . 3 50.70(18) no
P1 K1 Ba2 . . 3 51.3(3) no
P1 K1 K2 . . 4 64.6(2) no
P1 K1 Ba2 . . 4 64.8(4) no
P2 K1 O1 '3 544' . . 80.96(11) no
P2 K1 O2 '3 544' . . 132.73(11) no
P2 K1 O3 '3 544' . '1 545' 61.18(11) no
P2 K1 O11 '3 544' . . 69.50(10) no
P2 K1 O12 '3 544' . '1 545' 82.90(11) no
P2 K1 O5 '3 544' . '3 544' 25.09(9) no
P2 K1 O7 '3 544' . '3 544' 25.95(9) no
P2 K1 O8 '3 544' . . 119.0(5) no
P2 K1 Ti2 '3 544' . . 96.79(6) no
P2 K1 K2 '3 544' . '3 545' 110.2(2) no
P2 K1 Ba2 '3 544' . '3 545' 112.0(4) no
P2 K1 K2 '3 544' . 3 148.69(18) no
P2 K1 Ba2 '3 544' . 3 149.9(3) no
P2 K1 K2 '3 544' . 4 63.0(2) no
P2 K1 Ba2 '3 544' . 4 63.7(4) no
O1 K1 O2 . . . 52.45(14) no
O1 K1 O3 . . '1 545' 121.06(15) no
O1 K1 O11 . . . 55.15(15) no
O1 K1 O12 . . '1 545' 159.16(15) no
O1 K1 O5 . . '3 544' 55.90(13) no
O1 K1 O7 . . '3 544' 104.58(15) no
O1 K1 O8 . . . 90.2(4) no
O1 K1 Ti2 . . . 63.51(11) no
O1 K1 K2 . . '3 545' 147.7(2) no
O1 K1 Ba2 . . '3 545' 146.9(4) no
O1 K1 K2 . . 3 77.8(2) no
O1 K1 Ba2 . . 3 78.6(3) no
O1 K1 K2 . . 4 43.1(2) no
O1 K1 Ba2 . . 4 43.7(4) no
O2 K1 O3 . . '1 545' 133.33(15) no
O2 K1 O11 . . . 87.14(14) no
O2 K1 O12 . . '1 545' 144.19(15) no
O2 K1 O5 . . '3 544' 107.76(14) no
O2 K1 O7 . . '3 544' 156.94(15) no
O2 K1 O8 . . . 73.7(2) no
O2 K1 Ti2 . . . 71.44(11) no
O2 K1 K2 . . '3 545' 106.8(2) no
O2 K1 Ba2 . . '3 545' 105.1(4) no
O2 K1 K2 . . 3 38.0(2) no
O2 K1 Ba2 . . 3 38.0(3) no
O2 K1 K2 . . 4 75.8(2) no
O2 K1 Ba2 . . 4 75.5(4) no
O3 K1 O11 '1 545' . . 129.88(15) no
O3 K1 O12 '1 545' . '1 545' 60.45(15) no
O3 K1 O5 '1 545' . '3 544' 78.70(14) no
O3 K1 O7 '1 545' . '3 544' 56.25(14) no
O3 K1 O8 '1 545' . . 146.7(2) no
O3 K1 Ti2 '1 545' . . 153.88(11) no
O3 K1 K2 '1 545' . '3 545' 51.2(2) no
O3 K1 Ba2 '1 545' . '3 545' 52.9(4) no
O3 K1 K2 '1 545' . 3 150.1(2) no
O3 K1 Ba2 '1 545' . 3 148.9(3) no
O3 K1 K2 '1 545' . 4 78.7(2) no
O3 K1 Ba2 '1 545' . 4 78.2(4) no
O11 K1 O12 . . '1 545' 106.57(15) no
O11 K1 O5 . . '3 544' 58.48(13) no
O11 K1 O7 . . '3 544' 75.62(14) no
O11 K1 O8 . . . 56.9(6) no
O11 K1 Ti2 . . . 27.85(9) no
O11 K1 K2 . . '3 545' 156.9(2) no
O11 K1 Ba2 . . '3 545' 157.3(4) no
O11 K1 K2 . . 3 79.5(2) no
O11 K1 Ba2 . . 3 80.7(3) no
O11 K1 K2 . . 4 87.2(2) no
O11 K1 Ba2 . . 4 88.2(4) no
O12 K1 O5 '1 545' . '3 544' 107.57(14) no
O12 K1 O7 '1 545' . '3 544' 57.53(13) no
O12 K1 O8 '1 545' . . 86.2(2) no
O12 K1 Ti2 '1 545' . . 105.69(12) no
O12 K1 K2 '1 545' . '3 545' 51.7(2) no
O12 K1 Ba2 '1 545' . '3 545' 52.8(4) no
O12 K1 K2 '1 545' . 3 110.8(2) no
O12 K1 Ba2 '1 545' . 3 110.5(3) no
O12 K1 K2 '1 545' . 4 136.3(2) no
O12 K1 Ba2 '1 545' . 4 136.2(4) no
O5 K1 O7 '3 544' . '3 544' 50.05(13) no
O5 K1 O8 '3 544' . . 115.2(6) no
O5 K1 Ti2 '3 544' . . 85.73(10) no
O5 K1 K2 '3 544' . '3 545' 129.9(2) no
O5 K1 Ba2 '3 544' . '3 545' 131.5(4) no
O5 K1 K2 '3 544' . 3 129.3(2) no
O5 K1 Ba2 '3 544' . 3 130.4(3) no
O5 K1 K2 '3 544' . 4 45.1(2) no
O5 K1 Ba2 '3 544' . 4 46.1(4) no
O7 K1 O8 '3 544' . . 107.9(4) no
O7 K1 Ti2 '3 544' . . 97.72(11) no
O7 K1 K2 '3 544' . '3 545' 94.7(2) no
O7 K1 Ba2 '3 544' . '3 545' 96.4(4) no
O7 K1 K2 '3 544' . 3 146.8(2) no
O7 K1 Ba2 '3 544' . 3 147.7(3) no
O7 K1 K2 '3 544' . 4 88.0(2) no
O7 K1 Ba2 '3 544' . 4 88.6(4) no
O8 K1 Ti2 . . . 31.3(5) no
O8 K1 K2 . . '3 545' 108.6(6) no
O8 K1 Ba2 . . '3 545' 107.6(6) no
O8 K1 K2 . . 3 39.1(4) no
O8 K1 Ba2 . . 3 39.8(5) no
O8 K1 K2 . . 4 133.2(4) no
O8 K1 Ba2 . . 4 133.9(5) no
Ti2 K1 K2 . . '3 545' 139.8(2) no
Ti2 K1 Ba2 . . '3 545' 138.9(4) no
Ti2 K1 K2 . . 3 53.00(18) no
Ti2 K1 Ba2 . . 3 54.2(3) no
Ti2 K1 K2 . . 4 104.8(2) no
Ti2 K1 Ba2 . . 4 105.7(4) no
K2 K1 Ba2 '3 545' . '3 545' 1.8(4) no
K2 K1 K2 '3 545' . 3 100.0(3) no
K2 K1 Ba2 '3 545' . 3 98.8(4) no
K2 K1 K2 '3 545' . 4 113.7(3) no
K2 K1 Ba2 '3 545' . 4 112.7(4) no
Ba2 K1 K2 '3 545' . 3 98.2(4) no
Ba2 K1 Ba2 '3 545' . 3 97.1(5) no
Ba2 K1 K2 '3 545' . 4 114.1(4) no
Ba2 K1 Ba2 '3 545' . 4 113.1(5) no
K2 K1 Ba2 3 . 3 1.2(3) no
K2 K1 K2 3 . 4 112.4(3) no
K2 K1 Ba2 3 . 4 112.4(4) no
Ba2 K1 K2 3 . 4 112.7(4) no
Ba2 K1 Ba2 3 . 4 112.6(5) no
K2 K1 Ba2 4 . 4 1.1(4) no
K1 K2 Ba2 . . . 73(12) no
K1 K2 Ti1 . . . 53.96(19) no
K1 K2 P2 . . '3 544' 52.2(2) no
K1 K2 O4 . . '4 465' 76.5(3) no
K1 K2 O11 . . . 41.9(2) no
K1 K2 O7 . . '3 544' 43.7(2) no
K1 K2 K1 . . '3 544' 102.8(3) no
K1 K2 P1 . . '3 544' 144.2(4) no
K1 K2 O2 . . '3 544' 136.0(4) no
K1 K2 O8 . . '3 544' 78.8(5) no
K1 K2 K1 . . '3 554' 117.6(3) no
K1 K2 Ti2 . . '3 544' 96.6(3) no
K1 K2 O3 . . '3 544' 129.1(4) no
K1 K2 O12 . . '3 544' 80.4(3) no
K1 K2 K1 . . '4 455' 100.2(3) no
K1 K2 Ti1 . . '4 455' 133.8(4) no
K1 K2 O1 . . '4 455' 98.5(4) no
K1 K2 O5 . . '2 564' 146.1(4) no
Ba2 K2 Ti1 . . . 111(12) no
Ba2 K2 P2 . . '3 544' 120(12) no
Ba2 K2 O4 . . '4 465' 42(12) no
Ba2 K2 O11 . . . 80(12) no
Ba2 K2 O7 . . '3 544' 96(12) no
Ba2 K2 K1 . . '3 544' 136(12) no
Ba2 K2 P1 . . '3 544' 140(12) no
Ba2 K2 O2 . . '3 544' 124(12) no
Ba2 K2 O8 . . '3 544' 146(12) no
Ba2 K2 K1 . . '3 554' 121(12) no
Ba2 K2 Ti2 . . '3 544' 167(12) no
Ba2 K2 O3 . . '3 544' 157(12) no
Ba2 K2 O12 . . '3 544' 135(12) no
Ba2 K2 K1 . . '4 455' 33(12) no
Ba2 K2 Ti1 . . '4 455' 91(12) no
Ba2 K2 O1 . . '4 455' 69(12) no
Ba2 K2 O5 . . '2 564' 76(12) no
Ti1 K2 P2 . . '3 544' 55.4(2) no
Ti1 K2 O4 . . '4 465' 82.8(3) no
Ti1 K2 O11 . . . 31.30(18) no
Ti1 K2 O7 . . '3 544' 74.5(3) no
Ti1 K2 K1 . . '3 544' 98.5(3) no
Ti1 K2 P1 . . '3 544' 107.0(3) no
Ti1 K2 O2 . . '3 544' 124.8(4) no
Ti1 K2 O8 . . '3 544' 63.1(3) no
Ti1 K2 K1 . . '3 554' 65.7(2) no
Ti1 K2 Ti2 . . '3 544' 56.0(2) no
Ti1 K2 O3 . . '3 544' 82.3(3) no
Ti1 K2 O12 . . '3 544' 27.82(16) no
Ti1 K2 K1 . . '4 455' 143.8(4) no
Ti1 K2 Ti1 . . '4 455' 157.6(4) no
Ti1 K2 O1 . . '4 455' 147.4(5) no
Ti1 K2 O5 . . '2 564' 154.3(5) no
P2 K2 O4 '3 544' . '4 465' 126.0(4) no
P2 K2 O11 '3 544' . . 74.3(3) no
P2 K2 O7 '3 544' . '3 544' 27.37(16) no
P2 K2 K1 '3 544' . '3 544' 54.0(2) no
P2 K2 P1 '3 544' . '3 544' 92.0(3) no
P2 K2 O2 '3 544' . '3 544' 89.3(4) no
P2 K2 O8 '3 544' . '3 544' 27.2(5) no
P2 K2 K1 '3 544' . '3 554' 105.3(4) no
P2 K2 Ti2 '3 544' . '3 544' 53.7(2) no
P2 K2 O3 '3 544' . '3 544' 83.3(3) no
P2 K2 O12 '3 544' . '3 544' 61.6(3) no
P2 K2 K1 '3 544' . '4 455' 132.5(4) no
P2 K2 Ti1 '3 544' . '4 455' 109.8(4) no
P2 K2 O1 '3 544' . '4 455' 95.1(4) no
P2 K2 O5 '3 544' . '2 564' 143.9(5) no
O4 K2 O11 '4 465' . . 54.6(3) no
O4 K2 O7 '4 465' . '3 544' 118.2(5) no
O4 K2 K1 '4 465' . '3 544' 177.8(4) no
O4 K2 P1 '4 465' . '3 544' 135.8(4) no
O4 K2 O2 '4 465' . '3 544' 144.7(5) no
O4 K2 O8 '4 465' . '3 544' 145.5(5) no
O4 K2 K1 '4 465' . '3 554' 82.2(3) no
O4 K2 Ti2 '4 465' . '3 544' 129.9(4) no
O4 K2 O3 '4 465' . '3 544' 127.2(5) no
O4 K2 O12 '4 465' . '3 544' 97.9(4) no
O4 K2 K1 '4 465' . '4 455' 65.1(3) no
O4 K2 Ti1 '4 465' . '4 455' 118.4(4) no
O4 K2 O1 '4 465' . '4 455' 109.6(5) no
O4 K2 O5 '4 465' . '2 564' 88.1(4) no
O11 K2 O7 . . '3 544' 81.0(4) no
O11 K2 K1 . . '3 544' 126.1(4) no
O11 K2 P1 . . '3 544' 135.6(5) no
O11 K2 O2 . . '3 544' 156.1(6) no
O11 K2 O8 . . '3 544' 91.0(5) no
O11 K2 K1 . . '3 554' 78.3(3) no
O11 K2 Ti2 . . '3 544' 87.1(4) no
O11 K2 O3 . . '3 544' 110.1(5) no
O11 K2 O12 . . '3 544' 56.3(3) no
O11 K2 K1 . . '4 455' 112.5(4) no
O11 K2 Ti1 . . '4 455' 170.6(5) no
O11 K2 O1 . . '4 455' 136.8(5) no
O11 K2 O5 . . '2 564' 141.7(5) no
O7 K2 K1 '3 544' . '3 544' 60.7(3) no
O7 K2 P1 '3 544' . '3 544' 106.0(4) no
O7 K2 O2 '3 544' . '3 544' 92.4(4) no
O7 K2 O8 '3 544' . '3 544' 49.7(5) no
O7 K2 K1 '3 544' . '3 554' 132.5(5) no
O7 K2 Ti2 '3 544' . '3 544' 79.9(3) no
O7 K2 O3 '3 544' . '3 544' 105.9(4) no
O7 K2 O12 '3 544' . '3 544' 87.6(4) no
O7 K2 K1 '3 544' . '4 455' 105.3(4) no
O7 K2 Ti1 '3 544' . '4 455' 99.0(4) no
O7 K2 O1 '3 544' . '4 455' 73.1(4) no
O7 K2 O5 '3 544' . '2 564' 130.5(5) no
K1 K2 P1 '3 544' . '3 544' 45.61(16) no
K1 K2 O2 '3 544' . '3 544' 35.30(19) no
K1 K2 O8 '3 544' . '3 544' 35.6(2) no
K1 K2 K1 '3 544' . '3 554' 100.0(3) no
K1 K2 Ti2 '3 544' . '3 544' 52.14(17) no
K1 K2 O3 '3 544' . '3 544' 54.9(2) no
K1 K2 O12 '3 544' . '3 544' 84.0(3) no
K1 K2 K1 '3 544' . '4 455' 113.1(3) no
K1 K2 Ti1 '3 544' . '4 455' 60.6(2) no
K1 K2 O1 '3 544' . '4 455' 68.4(3) no
K1 K2 O5 '3 544' . '2 564' 91.5(3) no
P1 K2 O2 '3 544' . '3 544' 25.52(15) no
P1 K2 O8 '3 544' . '3 544' 65.4(5) no
P1 K2 K1 '3 544' . '3 554' 64.7(2) no
P1 K2 Ti2 '3 544' . '3 544' 52.8(2) no
P1 K2 O3 '3 544' . '3 544' 25.53(15) no
P1 K2 O12 '3 544' . '3 544' 79.9(3) no
P1 K2 K1 '3 544' . '4 455' 107.7(4) no
P1 K2 Ti1 '3 544' . '4 455' 53.5(2) no
P1 K2 O1 '3 544' . '4 455' 85.4(4) no
P1 K2 O5 '3 544' . '2 564' 64.2(3) no
O2 K2 O8 '3 544' . '3 544' 67.8(4) no
O2 K2 K1 '3 544' . '3 554' 89.9(3) no
O2 K2 Ti2 '3 544' . '3 544' 69.1(3) no
O2 K2 O3 '3 544' . '3 544' 49.6(3) no
O2 K2 O12 '3 544' . '3 544' 100.8(4) no
O2 K2 K1 '3 544' . '4 455' 91.3(4) no
O2 K2 Ti1 '3 544' . '4 455' 33.00(18) no
O2 K2 O1 '3 544' . '4 455' 60.4(3) no
O2 K2 O5 '3 544' . '2 564' 57.3(3) no
O8 K2 K1 '3 544' . '3 554' 88.3(5) no
O8 K2 Ti2 '3 544' . '3 544' 31.6(4) no
O8 K2 O3 '3 544' . '3 544' 56.9(5) no
O8 K2 O12 '3 544' . '3 544' 54.1(3) no
O8 K2 K1 '3 544' . '4 455' 143.8(5) no
O8 K2 Ti1 '3 544' . '4 455' 96.1(4) no
O8 K2 O1 '3 544' . '4 455' 97.6(5) no
O8 K2 O5 '3 544' . '2 564' 125.1(6) no
K1 K2 Ti2 '3 554' . '3 544' 56.9(2) no
K1 K2 O3 '3 554' . '3 544' 45.6(2) no
K1 K2 O12 '3 554' . '3 544' 45.5(2) no
K1 K2 K1 '3 554' . '4 455' 122.1(4) no
K1 K2 Ti1 '3 554' . '4 455' 108.0(3) no
K1 K2 O1 '3 554' . '4 455' 143.9(5) no
K1 K2 O5 '3 554' . '2 564' 89.3(4) no
Ti2 K2 O3 '3 544' . '3 544' 32.55(17) no
Ti2 K2 O12 '3 544' . '3 544' 33.09(17) no
Ti2 K2 K1 '3 544' . '4 455' 160.1(4) no
Ti2 K2 Ti1 '3 544' . '4 455' 102.1(3) no
Ti2 K2 O1 '3 544' . '4 455' 120.5(4) no
Ti2 K2 O5 '3 544' . '2 564' 116.1(4) no
O3 K2 O12 '3 544' . '3 544' 54.7(3) no
O3 K2 K1 '3 544' . '4 455' 130.1(4) no
O3 K2 Ti1 '3 544' . '4 455' 79.0(3) no
O3 K2 O1 '3 544' . '4 455' 110.0(5) no
O3 K2 O5 '3 544' . '2 564' 84.2(4) no
O12 K2 K1 '3 544' . '4 455' 162.0(5) no
O12 K2 Ti1 '3 544' . '4 455' 133.0(4) no
O12 K2 O1 '3 544' . '4 455' 151.5(6) no
O12 K2 O5 '3 544' . '2 564' 132.3(5) no
K1 K2 Ti1 '4 455' . '4 455' 58.3(2) no
K1 K2 O1 '4 455' . '4 455' 46.4(2) no
K1 K2 O5 '4 455' . '2 564' 46.0(2) no
Ti1 K2 O1 '4 455' . '4 455' 36.1(2) no
Ti1 K2 O5 '4 455' . '2 564' 34.26(19) no
O1 K2 O5 '4 455' . '2 564' 58.2(3) no
K1 Ba2 K2 . . . 106(12) no
K1 Ba2 Ti1 . . . 54.1(3) no
K1 Ba2 P2 . . '3 544' 52.4(4) no
K1 Ba2 O4 . . '4 465' 78.1(5) no
K1 Ba2 O11 . . . 42.5(4) no
K1 Ba2 O7 . . '3 544' 44.3(4) no
K1 Ba2 Ti2 . . . 53.9(3) no
K1 Ba2 K1 . . '3 544' 101.8(5) no
K1 Ba2 O2 . . '3 544' 134.6(8) no
K1 Ba2 O8 . . '3 544' 78.3(7) no
K1 Ba2 K1 . . '3 554' 116.9(6) no
K1 Ba2 O3 . . '3 544' 126.5(7) no
K1 Ba2 O12 . . '3 544' 80.0(6) no
K1 Ba2 K1 . . '4 455' 102.8(5) no
K1 Ba2 Ti1 . . '4 455' 135.1(6) no
K1 Ba2 O1 . . '4 455' 100.2(6) no
K1 Ba2 O5 . . '2 564' 150.2(7) no
K2 Ba2 Ti1 . . . 67(12) no
K2 Ba2 P2 . . '3 544' 58(12) no
K2 Ba2 O4 . . '4 465' 137(12) no
K2 Ba2 O11 . . . 97(12) no
K2 Ba2 O7 . . '3 544' 81(12) no
K2 Ba2 Ti2 . . . 118(12) no
K2 Ba2 K1 . . '3 544' 43(11) no
K2 Ba2 O2 . . '3 544' 54(12) no
K2 Ba2 O8 . . '3 544' 33(11) no
K2 Ba2 K1 . . '3 554' 57(11) no
K2 Ba2 O3 . . '3 544' 22(12) no
K2 Ba2 O12 . . '3 544' 43(12) no
K2 Ba2 K1 . . '4 455' 146(13) no
K2 Ba2 Ti1 . . '4 455' 87(12) no
K2 Ba2 O1 . . '4 455' 108(12) no
K2 Ba2 O5 . . '2 564' 102(12) no
Ti1 Ba2 P2 . . '3 544' 54.4(4) no
Ti1 Ba2 O4 . . '4 465' 83.3(6) no
Ti1 Ba2 O11 . . . 30.4(3) no
Ti1 Ba2 O7 . . '3 544' 73.4(6) no
Ti1 Ba2 Ti2 . . . 54.3(4) no
Ti1 Ba2 K1 . . '3 544' 95.9(5) no
Ti1 Ba2 O2 . . '3 544' 120.7(7) no
Ti1 Ba2 O8 . . '3 544' 61.5(5) no
Ti1 Ba2 K1 . . '3 554' 64.5(4) no
Ti1 Ba2 O3 . . '3 544' 79.8(5) no
Ti1 Ba2 O12 . . '3 544' 27.5(2) no
Ti1 Ba2 K1 . . '4 455' 146.9(7) no
Ti1 Ba2 Ti1 . . '4 455' 153.5(7) no
Ti1 Ba2 O1 . . '4 455' 146.9(9) no
Ti1 Ba2 O5 . . '2 564' 152.6(8) no
P2 Ba2 O4 '3 544' . '4 465' 127.0(8) no
P2 Ba2 O11 '3 544' . . 73.3(6) no
P2 Ba2 O7 '3 544' . '3 544' 26.7(2) no
P2 Ba2 Ti2 '3 544' . . 96.7(6) no
P2 Ba2 K1 '3 544' . '3 544' 52.6(3) no
P2 Ba2 O2 '3 544' . '3 544' 86.6(6) no
P2 Ba2 O8 '3 544' . '3 544' 26.6(5) no
P2 Ba2 K1 '3 544' . '3 554' 102.3(6) no
P2 Ba2 O3 '3 544' . '3 544' 80.2(5) no
P2 Ba2 O12 '3 544' . '3 544' 59.8(5) no
P2 Ba2 K1 '3 544' . '4 455' 134.3(7) no
P2 Ba2 Ti1 '3 544' . '4 455' 108.1(6) no
P2 Ba2 O1 '3 544' . '4 455' 94.3(7) no
P2 Ba2 O5 '3 544' . '2 564' 141.5(9) no
O4 Ba2 O11 '4 465' . . 56.1(5) no
O4 Ba2 O7 '4 465' . '3 544' 120.9(8) no
O4 Ba2 Ti2 '4 465' . . 31.1(3) no
O4 Ba2 K1 '4 465' . '3 544' 179.2(8) no
O4 Ba2 O2 '4 465' . '3 544' 146.2(10) no
O4 Ba2 O8 '4 465' . '3 544' 144.7(10) no
O4 Ba2 K1 '4 465' . '3 554' 82.3(6) no
O4 Ba2 O3 '4 465' . '3 544' 126.2(8) no
O4 Ba2 O12 '4 465' . '3 544' 98.0(7) no
O4 Ba2 K1 '4 465' . '4 455' 67.6(5) no
O4 Ba2 Ti1 '4 465' . '4 455' 121.3(8) no
O4 Ba2 O1 '4 465' . '4 455' 114.0(8) no
O4 Ba2 O5 '4 465' . '2 564' 90.8(7) no
O11 Ba2 O7 . . '3 544' 81.0(7) no
O11 Ba2 Ti2 . . . 25.2(3) no
O11 Ba2 K1 . . '3 544' 123.3(8) no
O11 Ba2 O2 . . '3 544' 151.1(9) no
O11 Ba2 O8 . . '3 544' 88.9(8) no
O11 Ba2 K1 . . '3 554' 77.2(6) no
O11 Ba2 O3 . . '3 544' 107.0(8) no
O11 Ba2 O12 . . '3 544' 55.2(5) no
O11 Ba2 K1 . . '4 455' 116.5(7) no
O11 Ba2 Ti1 . . '4 455' 175.6(8) no
O11 Ba2 O1 . . '4 455' 140.5(9) no
O11 Ba2 O5 . . '2 564' 145.0(10) no
O7 Ba2 Ti2 '3 544' . . 97.9(7) no
O7 Ba2 K1 '3 544' . '3 544' 59.0(4) no
O7 Ba2 O2 '3 544' . '3 544' 90.4(7) no
O7 Ba2 O8 '3 544' . '3 544' 48.5(6) no
O7 Ba2 K1 '3 544' . '3 554' 128.9(8) no
O7 Ba2 O3 '3 544' . '3 544' 102.2(7) no
O7 Ba2 O12 '3 544' . '3 544' 85.4(7) no
O7 Ba2 K1 '3 544' . '4 455' 107.8(7) no
O7 Ba2 Ti1 '3 544' . '4 455' 98.5(7) no
O7 Ba2 O1 '3 544' . '4 455' 73.5(6) no
O7 Ba2 O5 '3 544' . '2 564' 131.0(9) no
Ti2 Ba2 K1 . . '3 544' 148.3(7) no
Ti2 Ba2 O2 . . '3 544' 167.8(8) no
Ti2 Ba2 O8 . . '3 544' 114.1(8) no
Ti2 Ba2 K1 . . '3 554' 80.5(5) no
Ti2 Ba2 O3 . . '3 544' 121.2(7) no
Ti2 Ba2 O12 . . '3 544' 75.1(5) no
Ti2 Ba2 K1 . . '4 455' 93.6(5) no
Ti2 Ba2 Ti1 . . '4 455' 151.7(7) no
Ti2 Ba2 O1 . . '4 455' 131.2(7) no
Ti2 Ba2 O5 . . '2 564' 121.6(8) no
K1 Ba2 O2 '3 544' . '3 544' 34.2(3) no
K1 Ba2 O8 '3 544' . '3 544' 34.6(3) no
K1 Ba2 K1 '3 544' . '3 554' 97.1(4) no
K1 Ba2 O3 '3 544' . '3 544' 53.2(4) no
K1 Ba2 O12 '3 544' . '3 544' 81.2(5) no
K1 Ba2 K1 '3 544' . '4 455' 113.3(6) no
K1 Ba2 Ti1 '3 544' . '4 455' 59.4(3) no
K1 Ba2 O1 '3 544' . '4 455' 66.8(5) no
K1 Ba2 O5 '3 544' . '2 564' 89.7(6) no
O2 Ba2 O8 '3 544' . '3 544' 65.3(5) no
O2 Ba2 K1 '3 544' . '3 554' 87.4(5) no
O2 Ba2 O3 '3 544' . '3 544' 47.8(4) no
O2 Ba2 O12 '3 544' . '3 544' 96.8(6) no
O2 Ba2 K1 '3 544' . '4 455' 92.4(7) no
O2 Ba2 Ti1 '3 544' . '4 455' 33.0(3) no
O2 Ba2 O1 '3 544' . '4 455' 59.8(5) no
O2 Ba2 O5 '3 544' . '2 564' 56.7(5) no
O8 Ba2 K1 '3 544' . '3 554' 85.3(6) no
O8 Ba2 O3 '3 544' . '3 544' 54.4(6) no
O8 Ba2 O12 '3 544' . '3 544' 52.1(5) no
O8 Ba2 K1 '3 544' . '4 455' 144.0(8) no
O8 Ba2 Ti1 '3 544' . '4 455' 94.0(6) no
O8 Ba2 O1 '3 544' . '4 455' 95.8(8) no
O8 Ba2 O5 '3 544' . '2 564' 121.9(9) no
K1 Ba2 O3 '3 554' . '3 544' 44.5(3) no
K1 Ba2 O12 '3 554' . '3 544' 44.4(3) no
K1 Ba2 K1 '3 554' . '4 455' 123.3(7) no
K1 Ba2 Ti1 '3 554' . '4 455' 106.3(6) no
K1 Ba2 O1 '3 554' . '4 455' 142.2(9) no
K1 Ba2 O5 '3 554' . '2 564' 88.3(6) no
O3 Ba2 O12 '3 544' . '3 544' 52.5(4) no
O3 Ba2 K1 '3 544' . '4 455' 129.9(8) no
O3 Ba2 Ti1 '3 544' . '4 455' 77.4(5) no
O3 Ba2 O1 '3 544' . '4 455' 107.5(8) no
O3 Ba2 O5 '3 544' . '2 564' 82.4(6) no
O12 Ba2 K1 '3 544' . '4 455' 163.9(8) no
O12 Ba2 Ti1 '3 544' . '4 455' 129.1(7) no
O12 Ba2 O1 '3 544' . '4 455' 147.5(9) no
O12 Ba2 O5 '3 544' . '2 564' 129.3(8) no
K1 Ba2 Ti1 '4 455' . '4 455' 59.4(4) no
K1 Ba2 O1 '4 455' . '4 455' 48.3(4) no
K1 Ba2 O5 '4 455' . '2 564' 47.7(4) no
Ti1 Ba2 O1 '4 455' . '4 455' 35.9(3) no
Ti1 Ba2 O5 '4 455' . '2 564' 34.1(3) no
O1 Ba2 O5 '4 455' . '2 564' 59.1(6) no
K1 Ti1 K2 . . . 72.7(2) no
K1 Ti1 Ba2 . . . 71.4(3) no
K1 Ti1 O1 . . . 50.64(14) no
K1 Ti1 O11 . . . 52.72(15) no
K1 Ti1 O5 . . '3 544' 49.83(13) no
K1 Ti1 O6 . . '3 554' 123.05(15) no
K1 Ti1 O2 . . '2 664' 119.51(15) no
K1 Ti1 O12 . . '3 544' 122.53(17) no
K1 Ti1 K2 . . 4 65.6(2) no
K1 Ti1 Ba2 . . 4 63.4(4) no
K2 Ti1 Ba2 . . . 2.0(4) no
K2 Ti1 O1 . . . 121.4(3) no
K2 Ti1 O11 . . . 47.4(3) no
K2 Ti1 O5 . . '3 544' 73.6(3) no
K2 Ti1 O6 . . '3 554' 117.0(3) no
K2 Ti1 O2 . . '2 664' 140.2(3) no
K2 Ti1 O12 . . '3 544' 53.3(3) no
K2 Ti1 K2 . . 4 123.7(3) no
K2 Ti1 Ba2 . . 4 122.3(5) no
Ba2 Ti1 O1 . . . 119.7(4) no
Ba2 Ti1 O11 . . . 45.4(4) no
Ba2 Ti1 O5 . . '3 544' 74.0(4) no
Ba2 Ti1 O6 . . '3 554' 116.4(4) no
Ba2 Ti1 O2 . . '2 664' 142.1(4) no
Ba2 Ti1 O12 . . '3 544' 55.1(4) no
Ba2 Ti1 K2 . . 4 123.7(4) no
Ba2 Ti1 Ba2 . . 4 122.3(6) no
O1 Ti1 O11 . . . 82.7(2) no
O1 Ti1 O5 . . '3 544' 79.89(19) no
O1 Ti1 O6 . . '3 554' 87.1(2) no
O1 Ti1 O2 . . '2 664' 87.3(2) no
O1 Ti1 O12 . . '3 544' 172.6(2) no
O1 Ti1 K2 . . 4 48.3(3) no
O1 Ti1 Ba2 . . 4 46.9(4) no
O11 Ti1 O5 . . '3 544' 90.9(2) no
O11 Ti1 O6 . . '3 554' 91.2(2) no
O11 Ti1 O2 . . '2 664' 170.0(2) no
O11 Ti1 O12 . . '3 544' 94.8(2) no
O11 Ti1 K2 . . 4 117.6(3) no
O11 Ti1 Ba2 . . 4 115.4(4) no
O5 Ti1 O6 '3 544' . '3 554' 166.5(2) no
O5 Ti1 O2 '3 544' . '2 664' 86.7(2) no
O5 Ti1 O12 '3 544' . '3 544' 93.2(2) no
O5 Ti1 K2 '3 544' . 4 50.8(3) no
O5 Ti1 Ba2 '3 544' . 4 49.8(4) no
O6 Ti1 O2 '3 554' . '2 664' 89.0(2) no
O6 Ti1 O12 '3 554' . '3 544' 99.9(2) no
O6 Ti1 K2 '3 554' . 4 116.9(3) no
O6 Ti1 Ba2 '3 554' . 4 117.7(4) no
O2 Ti1 O12 '2 664' . '3 544' 95.0(2) no
O2 Ti1 K2 '2 664' . 4 54.0(3) no
O2 Ti1 Ba2 '2 664' . 4 56.2(4) no
O12 Ti1 K2 '3 544' . 4 128.5(3) no
O12 Ti1 Ba2 '3 544' . 4 129.5(4) no
K2 Ti1 Ba2 4 . 4 2.2(4) no
K1 Ti2 O3 . '1 545' '1 545' 48.67(13) no
K1 Ti2 O12 . '1 545' '1 545' 48.69(15) no
K1 Ti2 O7 . '1 545' '3 544' 57.76(15) no
K1 Ti2 K1 . '1 545' '1 545' 121.94(5) no
K1 Ti2 Ba2 . '1 545' '1 545' 158.7(3) no
K1 Ti2 O4 . '1 545' '4 455' 125.78(14) no
K1 Ti2 O11 . '1 545' '1 545' 129.89(17) no
K1 Ti2 O8 . '1 545' '1 545' 113.2(5) no
K1 Ti2 K2 . '1 545' '3 545' 61.7(2) no
O3 Ti2 O12 '1 545' '1 545' '1 545' 83.6(2) no
O3 Ti2 O7 '1 545' '1 545' '3 544' 85.8(2) no
O3 Ti2 K1 '1 545' '1 545' '1 545' 74.63(13) no
O3 Ti2 Ba2 '1 545' '1 545' '1 545' 133.4(4) no
O3 Ti2 O4 '1 545' '1 545' '4 455' 173.4(2) no
O3 Ti2 O11 '1 545' '1 545' '1 545' 92.6(2) no
O3 Ti2 O8 '1 545' '1 545' '1 545' 89.4(2) no
O3 Ti2 K2 '1 545' '1 545' '3 545' 51.5(3) no
O12 Ti2 O7 '1 545' '1 545' '3 544' 87.3(2) no
O12 Ti2 K1 '1 545' '1 545' '1 545' 124.38(15) no
O12 Ti2 Ba2 '1 545' '1 545' '1 545' 142.1(4) no
O12 Ti2 O4 '1 545' '1 545' '4 455' 89.8(2) no
O12 Ti2 O11 '1 545' '1 545' '1 545' 175.3(2) no
O12 Ti2 O8 '1 545' '1 545' '1 545' 84.1(6) no
O12 Ti2 K2 '1 545' '1 545' '3 545' 52.2(3) no
O7 Ti2 K1 '3 544' '1 545' '1 545' 139.32(16) no
O7 Ti2 Ba2 '3 544' '1 545' '1 545' 101.3(4) no
O7 Ti2 O4 '3 544' '1 545' '4 455' 93.4(2) no
O7 Ti2 O11 '3 544' '1 545' '1 545' 95.2(2) no
O7 Ti2 O8 '3 544' '1 545' '1 545' 170.6(5) no
O7 Ti2 K2 '3 544' '1 545' '3 545' 119.4(3) no
K1 Ti2 Ba2 '1 545' '1 545' '1 545' 70.4(4) no
K1 Ti2 O4 '1 545' '1 545' '4 455' 109.76(14) no
K1 Ti2 O11 '1 545' '1 545' '1 545' 51.60(16) no
K1 Ti2 O8 '1 545' '1 545' '1 545' 46.0(5) no
K1 Ti2 K2 '1 545' '1 545' '3 545' 74.9(2) no
Ba2 Ti2 O4 '1 545' '1 545' '4 455' 53.1(4) no
Ba2 Ti2 O11 '1 545' '1 545' '1 545' 41.2(4) no
Ba2 Ti2 O8 '1 545' '1 545' '1 545' 87.9(6) no
Ba2 Ti2 K2 '1 545' '1 545' '3 545' 139.0(4) no
O4 Ti2 O11 '4 455' '1 545' '1 545' 94.0(2) no
O4 Ti2 O8 '4 455' '1 545' '1 545' 90.5(2) no
O4 Ti2 K2 '4 455' '1 545' '3 545' 124.2(3) no
O11 Ti2 O8 '1 545' '1 545' '1 545' 93.1(6) no
O11 Ti2 K2 '1 545' '1 545' '3 545' 123.1(3) no
O8 Ti2 K2 '1 545' '1 545' '3 545' 51.8(5) no
K1 P1 O1 . . . 61.5(2) no
K1 P1 O2 . . . 56.7(2) no
K1 P1 O3 . . . 95.07(18) no
K1 P1 K2 . . 3 83.7(2) no
K1 P1 O4 . . . 155.91(18) no
O1 P1 O2 . . . 108.3(3) no
O1 P1 O3 . . . 112.3(3) no
O1 P1 K2 . . 3 143.1(3) no
O1 P1 O4 . . . 110.9(3) no
O2 P1 O3 . . . 105.9(3) no
O2 P1 K2 . . 3 54.4(3) no
O2 P1 O4 . . . 110.6(3) no
O3 P1 K2 . . 3 55.7(3) no
O3 P1 O4 . . . 108.6(2) no
K2 P1 O4 3 . . 105.9(3) no
K1 P2 K2 . '3 544' . 78.8(2) no
K1 P2 Ba2 . '3 544' . 77.0(4) no
K1 P2 O5 . '3 544' '3 544' 52.11(18) no
K1 P2 O7 . '3 544' '3 544' 59.0(2) no
K1 P2 O6 . '3 544' '3 544' 110.7(2) no
K1 P2 O8 . '3 544' '3 544' 138.8(5) no
K2 P2 Ba2 . '3 544' . 2.0(4) no
K2 P2 O5 . '3 544' '3 544' 88.7(3) no
K2 P2 O7 . '3 544' '3 544' 59.5(3) no
K2 P2 O6 . '3 544' '3 544' 162.1(3) no
K2 P2 O8 . '3 544' '3 544' 62.1(7) no
Ba2 P2 O5 . '3 544' '3 544' 88.4(5) no
Ba2 P2 O7 . '3 544' '3 544' 57.8(4) no
Ba2 P2 O6 . '3 544' '3 544' 162.2(5) no
Ba2 P2 O8 . '3 544' '3 544' 64.0(7) no
O5 P2 O7 '3 544' '3 544' '3 544' 108.1(3) no
O5 P2 O6 '3 544' '3 544' '3 544' 109.1(3) no
O5 P2 O8 '3 544' '3 544' '3 544' 111.2(3) no
O7 P2 O6 '3 544' '3 544' '3 544' 111.5(3) no
O7 P2 O8 '3 544' '3 544' '3 544' 106.5(7) no
O6 P2 O8 '3 544' '3 544' '3 544' 110.5(6) no
K1 O1 Ti1 . . . 94.23(18) no
K1 O1 P1 . . . 90.8(2) no
K1 O1 K2 . . 4 90.5(3) no
K1 O1 Ba2 . . 4 88.0(5) no
Ti1 O1 P1 . . . 130.7(3) no
Ti1 O1 K2 . . 4 95.6(3) no
Ti1 O1 Ba2 . . 4 97.2(5) no
P1 O1 K2 . . 4 133.3(4) no
P1 O1 Ba2 . . 4 132.0(6) no
K2 O1 Ba2 4 . 4 2.8(6) no
K1 O2 P1 . . . 95.2(2) no
K1 O2 Ti1 . . '2 665' 124.9(2) no
K1 O2 K2 . . 3 106.7(3) no
K1 O2 Ba2 . . 3 107.9(5) no
P1 O2 Ti1 . . '2 665' 132.0(3) no
P1 O2 K2 . . 3 100.0(4) no
P1 O2 Ba2 . . 3 101.7(5) no
Ti1 O2 K2 '2 665' . 3 93.1(3) no
Ti1 O2 Ba2 '2 665' . 3 90.8(5) no
K2 O2 Ba2 3 . 3 2.2(5) no
K1 O3 Ti2 . '1 545' '1 545' 97.05(17) no
K1 O3 P1 . '1 545' '1 545' 131.9(2) no
K1 O3 K2 . '1 545' '3 545' 83.1(3) no
K1 O3 Ba2 . '1 545' '3 545' 82.7(5) no
Ti2 O3 P1 '1 545' '1 545' '1 545' 130.0(3) no
Ti2 O3 K2 '1 545' '1 545' '3 545' 96.0(3) no
Ti2 O3 Ba2 '1 545' '1 545' '3 545' 96.9(5) no
P1 O3 K2 '1 545' '1 545' '3 545' 98.8(3) no
P1 O3 Ba2 '1 545' '1 545' '3 545' 98.4(5) no
K2 O3 Ba2 '3 545' '1 545' '3 545' 1.0(6) no
K2 O4 Ba2 . '4 465' . 1.7(5) no
K2 O4 Ti2 . '4 465' . 95.1(3) no
K2 O4 P1 . '4 465' '4 465' 126.6(3) no
Ba2 O4 Ti2 . '4 465' . 95.8(5) no
Ba2 O4 P1 . '4 465' '4 465' 126.4(5) no
Ti2 O4 P1 . '4 465' '4 465' 134.2(3) no
K1 O11 K2 . . . 99.7(3) no
K1 O11 Ba2 . . . 99.0(5) no
K1 O11 Ti1 . . . 95.8(2) no
K1 O11 Ti2 . . . 100.6(2) no
K2 O11 Ba2 . . . 2.9(5) no
K2 O11 Ti1 . . . 101.3(3) no
K2 O11 Ti2 . . . 116.0(4) no
Ba2 O11 Ti1 . . . 104.2(5) no
Ba2 O11 Ti2 . . . 113.6(6) no
Ti1 O11 Ti2 . . . 135.5(3) no
K1 O12 Ti2 . '1 545' '1 545' 96.50(18) no
K1 O12 K2 . '1 545' '3 545' 82.7(3) no
K1 O12 Ba2 . '1 545' '3 545' 82.8(5) no
K1 O12 Ti1 . '1 545' '3 545' 129.2(3) no
Ti2 O12 K2 '1 545' '1 545' '3 545' 94.7(3) no
Ti2 O12 Ba2 '1 545' '1 545' '3 545' 96.5(5) no
Ti2 O12 Ti1 '1 545' '1 545' '3 545' 133.5(3) no
K2 O12 Ba2 '3 545' '1 545' '3 545' 1.8(5) no
K2 O12 Ti1 '3 545' '1 545' '3 545' 98.9(3) no
Ba2 O12 Ti1 '3 545' '1 545' '3 545' 97.4(5) no
K1 O5 Ti1 . '3 544' . 97.04(17) no
K1 O5 P2 . '3 544' '3 544' 102.8(2) no
K1 O5 K2 . '3 544' 4 88.9(3) no
K1 O5 Ba2 . '3 544' 4 86.2(5) no
Ti1 O5 P2 . '3 544' '3 544' 132.9(3) no
Ti1 O5 K2 . '3 544' 4 94.9(3) no
Ti1 O5 Ba2 . '3 544' 4 96.0(5) no
P2 O5 K2 '3 544' '3 544' 4 127.3(4) no
P2 O5 Ba2 '3 544' '3 544' 4 127.2(6) no
K2 O5 Ba2 4 '3 544' 4 2.8(5) no
Ti1 O6 P2 . '3 554' '3 554' 135.2(3) no
K1 O7 K2 . '3 544' . 95.0(3) no
K1 O7 Ba2 . '3 544' . 93.5(5) no
K1 O7 Ti2 . '3 544' '1 545' 89.03(17) no
K1 O7 P2 . '3 544' '3 544' 95.1(2) no
K2 O7 Ba2 . '3 544' . 2.7(5) no
K2 O7 Ti2 . '3 544' '1 545' 136.1(4) no
K2 O7 P2 . '3 544' '3 544' 93.1(3) no
Ba2 O7 Ti2 . '3 544' '1 545' 133.9(5) no
Ba2 O7 P2 . '3 544' '3 544' 95.5(5) no
Ti2 O7 P2 '1 545' '3 544' '3 544' 130.1(3) no
K1 O8 Ti2 . . . 102.7(10) no
K1 O8 K2 . . 3 105.3(4) no
K1 O8 Ba2 . . 3 105.5(5) no
K1 O8 P2 . . . 119.3(5) no
Ti2 O8 K2 . . 3 96.7(3) no
Ti2 O8 Ba2 . . 3 98.0(5) no
Ti2 O8 P2 . . . 133.6(3) no
K2 O8 Ba2 3 . 3 1.4(5) no
K2 O8 P2 3 . . 90.7(11) no
Ba2 O8 P2 3 . . 89.4(11) no
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
K1 K2 . . 4.399(14) no
K1 Ba2 . . 4.36(3) no
K1 Ti1 . . 3.725(3) no
K1 Ti2 . '1 545' 3.603(2) no
K1 P1 . . 3.285(2) no
K1 P2 . '3 544' 3.544(3) no
K1 O1 . . 2.888(5) no
K1 O2 . . 2.756(5) no
K1 O3 . '1 545' 2.726(5) no
K1 O11 . . 2.979(5) no
K1 O12 . '1 545' 2.724(5) no
K1 O5 . '3 544' 2.868(5) no
K1 O7 . '3 544' 3.048(5) no
K1 O8 . . 2.755(11) no
K1 Ti2 . . 3.737(2) no
K1 K2 . '3 545' 3.786(14) no
K1 Ba2 . '3 545' 3.86(2) no
K1 K2 . 3 4.569(14) no
K1 Ba2 . 3 4.67(2) no
K1 K2 . 4 3.986(14) no
K1 Ba2 . 4 3.87(2) no
K2 Ba2 . . .14(3) no
K2 Ti1 . . 3.694(14) no
K2 P2 . '3 544' 3.382(14) no
K2 O4 . '4 465' 3.178(14) no
K2 O11 . . 2.771(15) no
K2 O7 . '3 544' 2.918(15) no
K2 P1 . '3 544' 3.557(14) no
K2 O2 . '3 544' 2.939(15) no
K2 O8 . '3 544' 2.99(2) no
K2 Ti2 . '3 544' 3.780(14) no
K2 O3 . '3 544' 2.973(14) no
K2 O12 . '3 544' 2.997(15) no
K2 Ti1 . '4 455' 3.630(14) no
K2 O1 . '4 455' 2.721(15) no
K2 O5 . '2 564' 2.823(15) no
Ba2 Ti1 . . 3.75(3) no
Ba2 P2 . '3 544' 3.45(3) no
Ba2 O4 . '4 465' 3.07(2) no
Ba2 O11 . . 2.75(3) no
Ba2 O7 . '3 544' 2.94(3) no
Ba2 Ti2 . . 3.82(2) no
Ba2 O2 . '3 544' 3.02(2) no
Ba2 O8 . '3 544' 3.11(3) no
Ba2 O3 . '3 544' 3.10(2) no
Ba2 O12 . '3 544' 3.10(3) no
Ba2 Ti1 . '4 455' 3.63(3) no
Ba2 O1 . '4 455' 2.67(3) no
Ba2 O5 . '2 564' 2.79(3) no
Ti1 O1 . . 2.149(5) no
Ti1 O11 . . 1.957(5) no
Ti1 O5 . '3 544' 2.051(5) no
Ti1 O6 . '3 554' 1.996(5) no
Ti1 O2 . '2 664' 1.979(5) no
Ti1 O12 . '3 544' 1.745(5) no
Ti2 O3 '1 545' '1 545' 2.045(5) no
Ti2 O12 '1 545' '1 545' 2.071(5) no
Ti2 O7 '1 545' '3 544' 1.974(5) no
Ti2 O4 '1 545' '4 455' 1.984(5) no
Ti2 O11 '1 545' '1 545' 1.776(5) no
Ti2 O8 '1 545' '1 545' 1.99(2) no
P1 O1 . . 1.525(5) no
P1 O2 . . 1.556(5) no
P1 O3 . . 1.551(5) no
P1 O4 . . 1.549(5) no
P2 O5 '3 544' '3 544' 1.541(5) no
P2 O7 '3 544' '3 544' 1.557(5) no
P2 O6 '3 544' '3 544' 1.533(5) no
P2 O8 '3 544' '3 544' 1.54(2) no
